# Research Article Phase-Field Simulations at the Atomic ... Phase-Field Simulations at the Atomic...

date post

14-Aug-2020Category

## Documents

view

0download

0

Embed Size (px)

### Transcript of Research Article Phase-Field Simulations at the Atomic ... Phase-Field Simulations at the Atomic...

Hindawi Publishing Corporation The Scientific World Journal Volume 2013, Article ID 564272, 8 pages http://dx.doi.org/10.1155/2013/564272

Research Article Phase-Field Simulations at the Atomic Scale in Comparison to Molecular Dynamics

Marco Berghoff, Michael Selzer, and Britta Nestler

Institute of Applied Materials, Karlsruhe Institute of Technology, 76133 Karlsruhe, Germany

Correspondence should be addressed to Marco Berghoff; marco.berghoff@kit.edu

Received 23 August 2013; Accepted 2 October 2013

Academic Editors: O. Balitskii and N. Sekido

Copyright ยฉ 2013 Marco Berghoff et al.This is an open access article distributed under the Creative CommonsAttribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.

Early solidification is investigated using two different simulation techniques: the molecular dynamics (MD) and the phase-field (PF) methods. While the first describes the evolution of a system on the basis of motion equations of particles, the second grounds on the evolution of continuous local order parameter field.The aim of this study is to probe the ability of themesoscopic phase-field method tomake predictions of growth velocity at the nanoscopic length scale. For this purpose the isothermal growth of a spherical crystalline cluster embedded in a melt is considered. The system in study is Ni modeled with the embedded atom method (EAM). The bulk and interfacial properties required in the PF method are obtained from MD simulations. Also the initial configuration obtained fromMDdata is used in the PF as input. Results for the evolution of the cluster volume at high andmoderate undercooling are presented.

1. Introduction

The phase-field is a powerful method to describe solidifi- cation phenomena [1, 2] on the mesoscopic length scale. It has been used to model homogeneous and heterogeneous nucleation, microstructure formation in solids, and motion of grain boundaries. The phase-field models includes formu- lations for pure substances [3], for multicomponent systems [4], and for polycrystalline structure [5] and solidification in eutectic [6, 7], peritectic [7], and monotectic [8] systems. Other simulation techniques for dendrite growth are cellular automata [9] and hybrid methods such as the multiscale diffusion Monte Carlo (DMC) [10, 11].

The phase-field method requires previous knowledge of the material properties of the system in study. The input includes bulk properties such as density, heat capacity and latent heat, and others such as interfacial and kinetic growth coefficients, being the latter properties which are hardly accessible in experiments. Here molecular simulations play a fundamental role, since they provide a link between an inter- action potential and all the required properties. Kinetic coefficients, interfacial free energies, and their dependence on the crystal orientation, of pure metals and alloys, can be

directly obtained from simulations of inhomogeneous liquid- crystal systems [12โ15].

There are previous phase-field studies in which the material parameters have been obtained frommolecular sim- ulations to model dendritic growth in pure Ni [16, 17], CO

2

hydrates [18], and binary alloys. In this work we compareMD and PF simulation results for the isothermal growth velocity of a nanoscopic spherical crystalline cluster of Ni embedded in the melt. For this purpose we use precise thermodynamic and kinetic data obtained from molecular dynamics and use equivalent initial configuration in the phase-field simula- tions.

2. Properties of Ni (EAM)

The properties of Ni obtained from molecular dynamic simulations are given in this section. The embedded atom potential of Foiles [19] is used. The thermal dependence of bulk properties is determined from independent simulations of equilibrated homogeneous systems at pressure ๐ = 0. Liquid phase is prepared by melting of an initial crystalline phase, by setting the temperature of the thermostat well above the melting temperature. Crystalline phase is obtained by

2 The Scientific World Journal

relaxation of the perfect crystalline phase. The samples are prepared in NpT simulation runs and the production in NVE ensemble.

Densities of the bulk phases are fitted to the function ๐ ๐ผ (๐) = ๐ + ๐ โ ๐ + ๐ โ ๐

2, for the fcc solid phase (๐ผ = s) ๐ = 8901.6 kg/m3, ๐ = โ0.20379 kg/m3 K, and ๐ = โ0.0000614202 kg/m3 K2 while for the liquid phase (๐ผ = โ) ๐ = 8992.26 kg/m3, ๐ = โ0.667037 kg/m3 K, and ๐ = 0.0000331612 kg/m3 K2.The parameters were obtained in the temperature intervals 1000K to 3000K for the liquid and 300K to 1900K for the solid. In both cases parts of the metastable phases are included in the fit procedure.

The latent heat is obtained from the difference between the enthalpy of the liquid and the solid and fitted to ๏ฟฝฬ๏ฟฝ

0 (๐) =

๐ + ๐ โ ๐ + ๐ โ ๐ 2 with ๐ = โ15980.2 J/kg, ๐ = 324.745 J/kg K,

and ๐ = โ0.0810984 J/kg K2. These values are determined in the range from 1000K to 1900K. The latent heat expressed in units of energy per volume of the solid phase is given by ๐ฟ s (๐) = ๏ฟฝฬ๏ฟฝ

0 (๐) โ ๐

s (๐).

The specific heat capacity at constant volume is given by ๐๐ผV (๐) = ๐ + ๐ โ ๐ where ๐ = 419.452 J/kg K and ๐ = 0.020388 J/kg K2 for the solid and ๐ = 563.024 J/kg K and ๐ = โ0.06952 J/kg K2 for the liquid.

The thermal diffusivity for themodel is 2.1โ 10โ7m2/s [20] while the experimental values range from 120 โ 10โ7m2/s [21] to the recent value 8.7โ 10โ7m2/s [22] (obtained inmicrograv- ity conditions).The value obtained from simulations is at least 4 times lower than that in experiments, and the difference is due to the electronic contribution to thermal transport in metals which are not accounted in classical molecular dynamics.

The melting temperature of the model is precisely esti- mated from simulations of inhomogeneous solid-liquid sys- tem at the point where the velocity of growth is zero. For the model ๐

๐ = 1748K.

The kinetic coefficient is estimated from linear relation- ship between planar growth velocity and undercooling close to coexistence. Growth velocities are obtained from inde- pendent simulations for the crystal orientations [100], [110], and [111]. The kinetic growth coefficient depends also on the orientation of the crystal. Its orientational dependence is represented here by the expansion

๐ (๐)

๐ 0

= 1 โ 3๐ ๐ + 4๐ ๐ ๐ + ๐ฟ

๐ (๐ + 30๐) (1)

with ๐ = ๐4 1 + ๐ 4

2 + ๐ 4

3 , ๐ = ๐6

1 + ๐ 6

2 + ๐ 6

3 , and ๐ = ๐2

1 ๐ 2

2 ๐ 2

3 .

๐ = (๐ 1 , ๐ 2 , ๐ 3 ) is the unit vector normal to the interface.

The parameter ๐ 0 is a value of the magnitude of the kinetic

coefficient; ๐ ๐ and ๐ฟ ๐ are the strength of the anisotropy of the

kinetic coefficient. The values for the model EAM F85 are ๐ 0

= 0.319205m/sK, ๐ ๐

= โ0.196511, and ๐ฟ ๐

= 0.230331, estimated from the kinetic coefficients for different crystal orientations; ๐

100 = 0.33m/sK, ๐

110 = 0.23m/sK, and ๐

111 =

0.12m/sK. The interfacial stiffness and interfacial free energy were

obtained from the analysis of capillary waves spectrum of large solid-liquid interfaces at coexistence (i.e., at ๐ = ๐

๐ for

๐ = 0). The orientational dependence of the interfacial free energy ๐พ is described by a cubic harmonic expansion

๐พ (๐)

๐พ 0

= 1 + ๐ 1 (๐ โ

3

5 ) + ๐ 2 (3๐ + 66๐ โ

17

7 )

+ ๐ 3 (5๐ 2 โ 16๐ โ

94

13 ๐ +

33

13 )

(2)

with ๐พ 0 being an orientational averaged value of the interfacial

free energy, while the coefficients ๐ ๐ describe the strength of

the anisotropy. Interfacial stiffness is defined as ๐พ ๐ผ๐ฝ

= ๐พ +

๐ 2 ๐พ/๐๐ ๐ผ ๐๐ ๐ฝ , where ๐

๐ผ and ๐ ๐ฝ indicate unit vectors tangent to

the interface plane [23]. The parameters of (2) are obtained from the system of equations for the stiffnesses ๐พ

๐ผ๐ฝ and

their numerical values are obtained from the analysis of the capillary waves spectrum [14]. Here we consider the crys- tal orientations [100], [110]

[110] , [110]

[001] , and [111]; the

interface energy for the [110] orientation depends on the parallel direction denoted by the subscripts. In respect to the four different interface energies we used a cubic harmonic expansion with four fitting parameters. Accurate values of these variables and parameters for the model EAM F85 are ๐พ 0

= 0.302 J/m2, ๐ 1

= 0.10191, ๐ 2

= โ0.00134, and ๐ 3

=

0.00876.

3. Phase-Field Model for Pure Material

Isothermal crystal growth for purematerial is modeled by the variables of the internal energy density ๐ and of two phase- fields 0 โค ๐s โค 1 (solid) and 0 โค ๐โ โค 1 (liquid). The phase-field variables fulfill the constraint ๐s + ๐โ = 1, so a single phase-field variable ๐ = ๐s is sufficient to describe the evolution of the phase boundaries in the system. Note that ๐ โ = 1 โ ๐. The variable ๐(๏ฟฝโ๏ฟฝ, ๐ก) denotes the local fraction at ๏ฟฝ

Recommended

*View more*